#------------------------------------------------------------------------------
#$Date: 2016-03-26 17:01:19 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180368 $
#$URL: svn://www.crystallography.net/cod/cif/7/20/37/7203771.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7203771
loop_
_publ_author_name
'León-Reina, Laura'
'Losilla, Enrique R.'
'Martínez-Lara, Maria'
'Bruque, Sebastián'
'Llobet, Anna'
'Sheptyakov, Denis V.'
'Aranda, Miguel A. G.'
_publ_section_title
;
 Interstitial oxygen in oxygen-stoichiometric apatites
;
_journal_issue                   25
_journal_name_full               'Journal of Materials Chemistry'
_journal_page_first              2489
_journal_paper_doi               10.1039/b503374h
_journal_volume                  15
_journal_year                    2005
_chemical_formula_sum            'La1.56 O4.35 Si'
_chemical_formula_weight         314.55
_chemical_name_systematic        ' ?'
_space_group_IT_number           176
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c'
_symmetry_space_group_name_H-M   'P 63/m'
_audit_creation_date             2005-03-07T16:15
_audit_creation_method           'from EXP file using GSAS2CIF'
_audit_update_record
' 2005-03-07T16:15 Initial CIF as created by GSAS2CIF'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                120.0
_cell_formula_units_Z            6
_cell_length_a                   9.81164(32)
_cell_length_b                   9.81164
_cell_length_c                   7.23354(24)
_cell_volume                     603.07(3)
_computing_structure_refinement  GSAS
_pd_block_id
2005-03-07T16:15|La933Si6_1173K|M.A.G.Aranda|Overall
_pd_phase_name
'from C:/Rietveld/Laura_Rietveld/Sinq_Dic2003/LaSiO/LaSiO_RT/LA933S'
_refine_ls_goodness_of_fit_all   1.71
_refine_ls_matrix_type           full
_refine_ls_number_parameters     87
_refine_ls_number_restraints     0
_refine_ls_shift/su_max          0.05
_refine_ls_shift/su_mean         0.01
_cod_data_source_file            b503374h.txt
_cod_data_source_block           La933Si6_1173K_overall
_cod_depositor_comments
;
The following automatic conversions were performed:
'_geom_angle_publ_flag' value 'N' changed to 'n' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (152
times).

'_geom_bond_publ_flag' value 'N' changed to 'n' according to
'/home/saulius/struct/CIF-dictionaries/cif_core.dic' dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29 (63 times).

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_original_cell_volume        603.06531
_cod_database_code               7203771
loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 +x,+y,+z
2 x-y,+x,+z+1/2
3 -y,x-y,+z
4 -x,-y,+z+1/2
5 y-x,-x,+z
6 +y,y-x,+z+1/2
-1 -x,-y,-z
-2 y-x,-x,-z+1/2
-3 +y,y-x,-z
-4 +x,+y,-z+1/2
-5 x-y,+x,-z
-6 -y,x-y,-z+1/2
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_thermal_displace_type
_atom_site_U_iso_or_equiv
_atom_site_symmetry_multiplicity
LA La1 0.23061(32) -0.0127(4) 0.25 1.0 Uani 0.01892 6
LA La2 0.3333 0.6667 -0.0012(7) 0.841 Uani 0.02666 4
SI SI 0.4007(6) 0.3718(6) 0.25 1.0 Uani 0.01898 6
O O1 0.3233(5) 0.4838(5) 0.25 1.0 Uani 0.04005 6
O O2 0.5908(4) 0.4715(6) 0.25 1.0 Uani 0.03481 6
O O3 0.3408(4) 0.2560(4) 0.07233(31) 1.0 Uani 0.04633 12
O O4 0.0 0.0 0.25 0.964(13) Uani 0.04 2
O O5 0.015(24) 0.246(20) 0.621(20) 0.0167(21) Uiso 0.03 12
loop_
_atom_type_symbol
_atom_type_number_in_cell
LA 9.364
SI 6.0
O 26.128
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 La1 O2 98.68(18) 5_555 . 3_655 n
O1 La1 O3 148.71(7) 5_555 . 1_555 n
O1 La1 O3 72.04(9) 5_555 . 6_555 n
O1 La1 O3 72.04(9) 5_555 . -3_555 n
O1 La1 O3 148.71(7) 5_555 . -4_556 n
O1 La1 O4 110.23(14) 5_555 . 1_555 n
O1 La1 O5 53(4) 5_555 . 4_554 n
O1 La1 O5 89(4) 5_555 . 5_555 n
O1 La1 O5 156.4(34) 5_555 . 6_554 n
O1 La1 O5 53(4) 5_555 . -1_556 n
O1 La1 O5 89(4) 5_555 . -2_556 n
O1 La1 O5 156.4(34) 5_555 . -3_556 n
O2 La1 O3 72.35(13) 3_655 . 1_555 n
O2 La1 O3 83.78(12) 3_655 . 6_555 n
O2 La1 O3 83.78(12) 3_655 . -3_555 n
O2 La1 O3 72.35(13) 3_655 . -4_556 n
O2 La1 O4 151.08(18) 3_655 . 1_555 n
O2 La1 O5 143(4) 3_655 . 4_554 n
O2 La1 O5 90(4) 3_655 . 5_555 n
O2 La1 O5 90(4) 3_655 . 6_554 n
O2 La1 O5 143(4) 3_655 . -1_556 n
O2 La1 O5 90(4) 3_655 . -2_556 n
O2 La1 O5 90(4) 3_655 . -3_556 n
O3 La1 O3 133.97(15) 1_555 . 6_555 n
O3 La1 O3 77.14(6) 1_555 . -3_555 n
O3 La1 O3 58.49(13) 1_555 . -4_556 n
O3 La1 O4 82.52(10) 1_555 . 1_555 n
O3 La1 O5 117.1(34) 1_555 . 4_554 n
O3 La1 O5 120(4) 1_555 . 5_555 n
O3 La1 O5 20(4) 1_555 . 6_554 n
O3 La1 O5 145(4) 1_555 . -1_556 n
O3 La1 O5 61(4) 1_555 . -2_556 n
O3 La1 O5 54.9(34) 1_555 . -3_556 n
O3 La1 O3 139.53(19) 6_555 . -3_555 n
O3 La1 O3 77.14(6) 6_555 . -4_556 n
O3 La1 O4 104.69(11) 6_555 . 1_555 n
O3 La1 O5 105.8(34) 6_555 . 4_554 n
O3 La1 O5 20(4) 6_555 . 5_555 n
O3 La1 O5 130.9(34) 6_555 . 6_554 n
O3 La1 O5 65(4) 6_555 . -1_556 n
O3 La1 O5 159(4) 6_555 . -2_556 n
O3 La1 O5 87.5(35) 6_555 . -3_556 n
O3 La1 O3 133.97(15) -3_555 . -4_556 n
O3 La1 O4 104.69(11) -3_555 . 1_555 n
O3 La1 O5 65(4) -3_555 . 4_554 n
O3 La1 O5 159(4) -3_555 . 5_555 n
O3 La1 O5 87.5(35) -3_555 . 6_554 n
O3 La1 O5 105.8(34) -3_555 . -1_556 n
O3 La1 O5 20(4) -3_555 . -2_556 n
O3 La1 O5 130.9(34) -3_555 . -3_556 n
O3 La1 O4 82.52(10) -4_556 . 1_555 n
O3 La1 O5 145(4) -4_556 . 4_554 n
O3 La1 O5 61(4) -4_556 . 5_555 n
O3 La1 O5 54.9(34) -4_556 . 6_554 n
O3 La1 O5 117.1(34) -4_556 . -1_556 n
O3 La1 O5 120(4) -4_556 . -2_556 n
O3 La1 O5 20(4) -4_556 . -3_556 n
O4 La1 O5 62(4) 1_555 . 4_554 n
O4 La1 O5 90(4) 1_555 . 5_555 n
O4 La1 O5 63(4) 1_555 . 6_554 n
O4 La1 O5 62(4) 1_555 . -1_556 n
O4 La1 O5 90(4) 1_555 . -2_556 n
O4 La1 O5 63(4) 1_555 . -3_556 n
O5 La1 O5 111(6) 4_554 . 5_555 n
O5 La1 O5 108(7) 4_554 . 6_554 n
O5 La1 O5 43(7) 4_554 . -1_556 n
O5 La1 O5 68(5) 4_554 . -2_556 n
O5 La1 O5 125(6) 4_554 . -3_556 n
O5 La1 O5 112(6) 5_555 . 6_554 n
O5 La1 O5 68(5) 5_555 . -1_556 n
O5 La1 O5 179(8) 5_555 . -2_556 n
O5 La1 O5 69(4) 5_555 . -3_556 n
O5 La1 O5 125(6) 6_554 . -1_556 n
O5 La1 O5 69(4) 6_554 . -2_556 n
O5 La1 O5 44(7) 6_554 . -3_556 n
O5 La1 O5 111(6) -1_556 . -2_556 n
O5 La1 O5 108(7) -1_556 . -3_556 n
O5 La1 O5 112(6) -2_556 . -3_556 n
La2 La2 La2 179.9604 -2_565 . -2_566 n
La2 La2 O1 136.11(11) -2_565 . 1_555 n
La2 La2 O1 136.11(11) -2_565 . 3_665 n
La2 La2 O1 136.15(11) -2_565 . 5_565 n
La2 La2 O2 45.70(13) -2_565 . 2_554 n
La2 La2 O2 45.69(13) -2_565 . 4_664 n
La2 La2 O2 45.68(13) -2_565 . 6_564 n
La2 La2 O1 43.88(11) -2_566 . 1_555 n
La2 La2 O1 43.87(11) -2_566 . 3_665 n
La2 La2 O1 43.89(11) -2_566 . 5_565 n
La2 La2 O2 134.33(13) -2_566 . 2_554 n
La2 La2 O2 134.29(13) -2_566 . 4_664 n
La2 La2 O2 134.31(13) -2_566 . 6_564 n
O1 La2 O1 73.77(18) 1_555 . 3_665 n
O1 La2 O1 73.78(18) 1_555 . 5_565 n
O1 La2 O2 124.18(11) 1_555 . 2_554 n
O1 La2 O2 92.72(8) 1_555 . 4_664 n
O1 La2 O2 154.26(13) 1_555 . 6_564 n
O1 La2 O1 73.78(18) 3_665 . 5_565 n
O1 La2 O2 154.30(13) 3_665 . 2_554 n
O1 La2 O2 124.16(11) 3_665 . 4_664 n
O1 La2 O2 92.74(8) 3_665 . 6_564 n
O1 La2 O2 92.76(8) 5_565 . 2_554 n
O1 La2 O2 154.28(13) 5_565 . 4_664 n
O1 La2 O2 124.20(11) 5_565 . 6_564 n
O2 La2 O2 76.59(20) 2_554 . 4_664 n
O2 La2 O2 76.59(20) 2_554 . 6_564 n
O2 La2 O2 76.58(20) 4_664 . 6_564 n
O1 SI O2 112.4(5) 1_555 . 1_555 n
O1 SI O3 110.37(25) 1_555 . 1_555 n
O1 SI O3 110.37(25) 1_555 . -4_556 n
O1 SI O5 91(7) 1_555 . 6_554 n
O1 SI O5 91(7) 1_555 . -3_556 n
O2 SI O3 109.19(28) 1_555 . 1_555 n
O2 SI O3 109.19(28) 1_555 . -4_556 n
O2 SI O5 140(6) 1_555 . 6_554 n
O2 SI O5 140(6) 1_555 . -3_556 n
O3 SI O3 105.1(4) 1_555 . -4_556 n
O3 SI O5 31(6) 1_555 . 6_554 n
O3 SI O5 90(5) 1_555 . -3_556 n
O3 SI O5 90(5) -4_556 . 6_554 n
O3 SI O5 31(6) -4_556 . -3_556 n
O5 SI O5 65(10) 6_554 . -3_556 n
La1 O1 La2 103.95(12) 3_555 . 1_555 n
La1 O1 La2 103.96(12) 3_555 . -2_566 n
La1 O1 SI 96.39(29) 3_555 . 1_555 n
La2 O1 La2 92.24(23) 1_555 . -2_566 n
La2 O1 SI 128.25(13) 1_555 . 1_555 n
La2 O1 SI 128.23(13) -2_566 . 1_555 n
La1 O2 La2 114.75(11) 5_665 . 2_655 n
La1 O2 La2 114.74(11) 5_665 . -1_665 n
La1 O2 SI 125.4(4) 5_665 . 1_555 n
La2 O2 La2 88.62(26) 2_655 . -1_665 n
La2 O2 SI 103.36(25) 2_655 . 1_555 n
La2 O2 SI 103.38(25) -1_665 . 1_555 n
La1 O3 La1 114.41(18) 1_555 . 2_554 n
La1 O3 SI 97.97(19) 1_555 . 1_555 n
La1 O3 O5 72(12) 1_555 . 6_554 n
La1 O3 SI 143.28(25) 2_554 . 1_555 n
La1 O3 O5 93(9) 2_554 . 6_554 n
SI O3 O5 81(10) 1_555 . 6_554 n
La1 O4 La1 120.0 1_555 . 3_555 n
La1 O4 La1 120.0 1_555 . 5_555 n
La1 O4 La1 120.0 3_555 . 5_555 n
La1 O5 La1 112(7) 2_555 . 3_555 n
La1 O5 La1 107(6) 2_555 . 4_555 n
La1 O5 SI 100(8) 2_555 . 2_555 n
La1 O5 O3 88(13) 2_555 . 2_555 n
La1 O5 La1 111(6) 3_555 . 4_555 n
La1 O5 SI 123(8) 3_555 . 2_555 n
La1 O5 O3 67(8) 3_555 . 2_555 n
La1 O5 SI 103(8) 4_555 . 2_555 n
La1 O5 O3 164(16) 4_555 . 2_555 n
SI O5 O3 68(10) 2_555 . 2_555 n
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
La1 La1 4.032(4) . 3_555 n
La1 La1 4.032(4) . 5_555 n
La1 SI 3.274(7) . 1_555 n
La1 SI 3.359(6) . 5_555 n
La1 O1 2.769(6) . 5_555 n
La1 O2 2.537(5) . 3_655 n
La1 O3 2.631(4) . 1_555 n
La1 O3 2.4850(26) . 6_555 n
La1 O3 2.4850(26) . -3_555 n
La1 O3 2.631(4) . -4_556 n
La1 O4 2.3276(26) . 1_555 n
La1 O5 2.53(18) . 4_554 n
La1 O5 2.69(14) . 5_555 n
La1 O5 2.50(19) . 6_554 n
La1 O5 2.53(18) . -1_556 n
La1 O5 2.69(14) . -2_556 n
La1 O5 2.50(19) . -3_556 n
La2 La2 3.600(10) . -2_565 n
La2 La2 3.634(10) . -2_566 n
La2 SI 3.343(5) . 2_554 n
La2 SI 3.344(5) . 4_664 n
La2 SI 3.343(5) . 6_564 n
La2 O1 2.521(4) . 1_555 n
La2 O1 2.521(4) . 3_665 n
La2 O1 2.520(4) . 5_565 n
La2 O2 2.576(4) . 2_554 n
La2 O2 2.577(4) . 4_664 n
La2 O2 2.576(4) . 6_564 n
La2 O3 2.9391(31) . -1_665 n
La2 O3 2.9381(31) . -3_565 n
La2 O3 2.9388(31) . -5_555 n
SI La1 3.274(7) . 1_555 n
SI La1 3.359(6) . 3_555 n
SI La2 3.343(5) . 2_655 n
SI La2 3.344(5) . -1_665 n
SI O1 1.618(7) . 1_555 n
SI O2 1.616(5) . 1_555 n
SI O3 1.619(4) . 1_555 n
SI O3 1.619(4) . -4_556 n
SI O5 1.73(16) . 6_554 n
SI O5 1.73(16) . -3_556 n
O1 La1 2.769(6) . 3_555 n
O1 La2 2.521(4) . 1_555 n
O1 La2 2.521(4) . -2_566 n
O1 SI 1.618(7) . 1_555 n
O2 La1 2.537(5) . 5_665 n
O2 La2 2.576(4) . 2_655 n
O2 La2 2.577(4) . -1_665 n
O2 SI 1.616(5) . 1_555 n
O3 La1 2.631(4) . 1_555 n
O3 La1 2.4850(26) . 2_554 n
O3 La2 2.9391(31) . -1_665 n
O3 SI 1.619(4) . 1_555 n
O3 O5 0.91(17) . 6_554 n
O4 La1 2.3276(26) . 1_555 n
O4 La1 2.3276(26) . 3_555 n
O4 La1 2.3276(26) . 5_555 n
O5 La1 2.50(19) . 2_555 n
O5 La1 2.69(14) . 3_555 n
O5 La1 2.53(18) . 4_555 n
O5 SI 1.73(16) . 2_555 n
O5 O3 0.91(17) . 2_555 n
O5 O5 1.86(29) . -4_557 n
loop_
_pd_block_diffractogram_id
2005-03-07T16:15|La933Si6_1173K_H_01|M.A.G.Aranda|hrpt_npd
loop_
_pd_phase_block_id
2005-03-07T16:15|La933Si6_1173K_phase1|M.A.G.Aranda||
2005-03-07T16:15|La933Si6_1173K_phase2|M.A.G.Aranda||
